**Optica Applicata, Vol. X , N o. 4, 1980**

**Temperature dependence of the **

**R 0A**

**R 0A**

** product for **

**photovoltaic PbTe detectors**

**Antoni Rogalski, Jabosław Rutkowski**

**In stitu te of Technical Physics, M ilitary Technical A ca d em y , W a rsaw , Poland.**

**In the paper the lim itin g values of the B 0A product h ave been calculated for ****diffusion p -n P b T e junctions within the tem perature range 7 7 -3 0 0 K . T he ****influence of the diffusion current (for the radiative and Auger recom bination) **
**and the generation-recom bination current upon B 0A is discussed. The calculations ****h ave been carried out for optim um doping concentrations, for which the contri**
**bution of tunnel current com ponent m a y be neglected. A lso the calculations **
**of B****q****A**** for the Sch ottky junction are performed. T h e results of calculations are **
**com pared w ith the experim ental data reported b y other authors. A satisfactory **
**consistence has been achieved for p -n junctions. A n attem p t was m ade to explain ****the divergences which appear for S ch ottky junctions. The working conditions for **
**ph otovoltaic detectors, the d etectivity of which is lim ited b y the background **
**radiation, were determined.**

**Introduction**

The semiconductor lead chalcogenide compounds find a wide application in optoelectronics as detectors and sources (lasers) of infrared radiation. Due to the difficulties in the production of materials of low concentration and the short lifetime of the carriers in those compounds the main effort is directed toward the production of the photovoltaic detectors.

PbTe is a semiconductor on the base of which the photovoltaic detectors
*(p-n junction [1-8], and Schottky junctions [9-12]) are produced for the *
spectral range 3-5 [im. In the paper [13] the influence of the doping con
*centration on the R 0A product (differential resistance — zero-volt bias — *
*times the junction area) has been analysed for the abrupt p-n PbTe junc*
tions.

*In the present paper the limiting values of R0A for the abrupt p-n *
PbTe junction were determined for the temperature range 77-300 K. The
calculations were carried out for the optimum doping concentration for
which the carrier tunnelling may be neclected. The influence of the diffusion
and generation-recombination current in the depletion layer upon the
*R 0A product has been considered. A comparison of the abrupt p-n junction *
with that of Schottky type is made. The results of considerations are
confronted with the experimental data reported by other authors.

**Abrupt ****p -n**** junction**

The total density of dark current flowing through the junction may be written in the form

**436** **A . Rogalski, J. Ru t k o w s k i**

where the particular components denote respectively: diffusion current
density, generation-recombination current density in the depletion layer,,
tunelling current density and leakage current density. For the optimum
doping concentrations, considered in this paper, the contribution of the
*tunnelling component may be neglected. The Z component may be caused *
by both volume and surfaces defects of the material. For a suitable techno
*logy and design of the diode the influence of the Jz component is unessen*
tial.

*The R 0A product determined by the diffusion current in the case *
of radiative recombination is [14]:

*f.i * — average values of the mobility of electrons and holes,

*ni * — intrinsic concentration,

*q * — electron charge,

*R * — coefficient of radiative recombination.

The intrinsic concentration is determined by the formula [15]:

*where mdp and m*dn denote the density-of-states effective masses, and *
*Eg — energy gap. The formula (3) is valid for Egy k T , being fulfilled *
in the case of PbTe. The values of density-of-effective masses state may be
determined when knowing the longitudinal and transversal components
*of the effective mass, since md = A 2/3 [m* m*2]1/3. For the lead chalco- *
genides the number of equivalent extremes in the conduction and valence
bands is equal to 4.

Due to the mirror symmetry of the conduction and valence bands the values of effective masses of the electrons and holes are close to each

*other m* * In this case the coefficient of radiative recombination

*JR = JRn = Rp, and, as it is shown in [16], amounts to*

*where n denotes the refractive index, K = m* jm* is the coefficient of *
*anisotropy of effective masses, m0 is the mass of free electron. The mass m* *
*may be determined from the formula m* = [1/3(2 /m * + l/m * )]-1 . In *
*the formula (4) kT and E g are expressed in electronovolts. For the Auger *
recombination [14}:

**(2)**

*where net — np/(n+2V np+p) — effective doping concentration,*

**nt**

**nt**

** = **

**2**

**[**

**2**

**TtkTI^f2 [m*dnm*dp f ^ x p [ - E gl2kT^**

**TtkTI^f2 [m*dnm*dp f ^ x p [ - E gl2kT^**

**(3)**

*R =*l x l O - 15^ 2

**( 4 )**

*[k T f l2K 112 [2 + 1 I K ? 12 [m* I m0]512 ’*

*(Ro^ )a =*

*(kT)112*

**(5)**

*2 q312 n2 p1/2 C112 **

**Temperature dependence o f the R^A product...****437**

*The Auger recombination coefficient G = Gn = Cp has the form [17]:*

*G =* *1 * *N' q4 *

(2tt*)1/2 N 2 el* *[JcT]ll2E~712*

*h3*

*1/2 exp _{L } _{2&T J}

*ml * *mt* **(6)**

*where £M is a high-frequency dielectric constant, and N' — 3 is the *
number of valleys, to which the energy scatter from a given valley may
occur.

*The RqA product, denoted by the generation-recombination region of *

the depletion layer in the abrupt junction, is [18]:

*(R,0A )gr —* . r r

*-«».·(2 ..) w Vn“ ’* **(7)**

*where es denotes the static dielectric constant and net = n p K n + p) is the *
effective concentration.

In the formula (7) r0 (the time determining the recomination by the Shockley-Read centers) is a parameter difficult to determine. The Shockley- Read centers cannot be of hydrogen-like nature because great dielectric constant would cause their shift toward the band edge and then their influence on the lifetime would be quite small. It can be only suggested that these centres are positioned within the energy gap and are not connec ted with the electrically active defects [18].

**Schottky’s junction**

*The product R 0A for the Schottky’s junction is determined by [19]:*

*= 'kq A ^ 6XP [ w ] ’ * <8>

*where cpB denotes the barrier height and A* is the Richardson constant.*
*The formula (8) is valid for an ideal M S junction under the following *
assumptions: i) the barrier height is much greater than kT, and ii) the
collisions in the barrier region and such phenomena as the influence of
the image forces, tunnelling through the upper part of the barrier and
penetration of the barrier by the surface states, are neglected.

In the papers [20] and [12] it has been pointed out that in the case of
a metal-semiconductor junction with narrow energy gap and for the hole-
*type conduction the effective barrier height <pB exceeds slightly the *
energy gap and is independent of the work function in metal.

*Assuming cpB = Eg, the expression (8) takes the form*

*h3 * 1 *r E gl *

**i - q - k ****m*** * T* CXP

**L **

**k**

**T***'*

**\****438** **A. Rogalski, J. Rutkowski**

**Numerical results o f calculations and discussion**

*The temperature dependence of the B 0A product, defined by the Auger *
radiative recombination and the depletion layer, was estimated from the
formulae (2), (5), and (7). The calculations were carried out for optimum
*effective doping concentrations for which the B 0A product takes the *
maximum value. From the calculation performed in the work [13] it follows
that, for instance, at the temperatures 77, 200, and 300 K these concen
trations are equal respectively to 6 xlO 23 m“ 3, 3 xlO 24 m~3, and 1 xlO 25
*m-3 . If this concentration is exceeded an abrupt drop of B 0A occurs, which *
is caused by the tunnel current. It has been assumed in the calculation that
the energy gap in PbTe changes with the temperature in accordance with
*the formula Ea(T) = 0.19+4.1 x lO ” 4 T (expressed in electronovolts) [21]. *
The effective mass values were determined according to [22], taking the
average values of the effective masses of electrons and holes, and assuming
that the effective masses change proportionally to the energy gap width.
The above approximation is justified by the results of both theoretical
and experimental investigations of the band structure of the lead chalco-
genide compounds [16, 20]. The values of the effective mass, the anisotropy
*coefficient K, the carrier mobility p, the refractive index n, the static *

*dielectric constant es, and high frequency dielectric constant * , assumed

according to [21, 23], were approximated in the temperature range 77-300
K. The material parameters of PbTe for the chosen temperatures are
*collected in table. In the calculations of (B 0A )GR it has been assumed that*

**T a b l e**
**M aterial parameters of P b T e**
**T**
**[K ]** **B 9 [e V ]***m * j m 0* *m *t / m 0* *m *d l m o* *m * J m g*
**1**
**K**

**4 w ]**

**n****£oo**

**77**

**0.22**

**0.3 1 4**

**0.0 2 6**

**0.037**

**0.019**

**12**

**2 .00**

**6.4**

**400**

**38**

**200**

**0.27**

**0.391**

**0.033**

**0.047**

**0.0 2 4**

**12**

**0 .3 0**

**6.2**

**400**

**36**

**300**

**0.32**

**0.4 6 3**

**0.039**

**0 .0 5 6**

**0.0 2 8**

**12**

**0.13**

**6.0**

**400**

**34**

*Tg = 10-8 s. For lead chalcogenides the time of similar order of magnitudes *
is often assumed [18, 20].

*The results of calculations for the p-n junction are shown in fig. 1. In *
the temperature of 77 K the main contribution to the current flow through
the junction comes from the generation-recombination current of the deple
*tion layer for which ( B0A ) GR is the smallest. The theoretical evaluation *
for the radiative and Auger recombinations give the values greater by four
orders of magnitude. As the temperature increases the influence of deple
tion layer decreases, while in the temperature range above 150 K it is the
*Auger process which determines the values of B 0A.*

The respective calculations
for an ideal Schottky junction
were carried out by taking ad
vantage of the formula (9) and
are represented graphically in
fig. 2. In the same figure the
temperature dependence of the
*resultant B 0A of the p-n junc*
tion, i.e.

**(RoA**

**(RoA**

*) - 1*

= **(BoA)z**

**(BoA)z**

*1*

### +

**{RoAL**· 1

**( R****o****A )****qr**is given for comparison.

From the comparison of the theoretical curves with the ex perimental data (seefig. 2) it may be seen that a satisfactory con sistence has been achieved foi*

**F ig. ** **1. ** **Tem perature ** **dependence **
**of ** **the ** **R 0A****product ** **determ ined **
**b y the radiative recom bination, A u **
**ger recom bination and the space **
**charge region for the p -n junction**

*p-n junction in a wide temperature range. It should be noted *
that the authors of the works, from which the experimental data have
been taken to draw the points in fig. 2, do not report on doping concentra
*tions on both sides of the junction. The experimental values for M S *
junctions are found only for the temperature of 77 K, deviation from the
value calculated for this temperature is very high amounting to four
orders of magnitude. This divergence seems to be due to the use of the
formula (9) which does not take account of additional processes occurring
in the metal-semi conductor junction with narrow energy gap and hole-type
conduction. The scheme of energy bands for such a junction has been
proposed by **Ki l l** and **W** **a l p o l e [ 2 0 ] **and is shown in fig. **3 , **where three

regions may be distinguished: inversion, depletion, and bulk ones. In the
ideal junction only processes (a), i.e. the hole emission from the Fermi
*level in metal to the valence band for hv — <pBc are considered. No account *
is taken of the excitation of electron-hole pairs in the inversion region
(processes (b)), and of the band-band transmissions for electron-hole
pairs in the depletion region (processes (c)). The last transitions are of
particular importance, because the depletion layer is wide due to high
dielectric constant. According to the authors of the work [9] the barrier
*height <pBC for holes is considerably lowered to take the value <pBE slightly*

**Temperature dependence o f the B 0A p rodu ct...****439**

**300 200 ** **100 ** **77**

Fy
\|
i?
m
2|
**440** **A. Rogalski, J. Rutkowski**
t|k|
**300 200 ** **100 ** **77**

*exceeding the energy gap Eg. *
Since for the holes of kinetic
*energy slightly exceeding Eg the *
narrow end of the harrier is trans
parent dne to tunnelling ef
*fects, the effective barrier cpBE *
(determined, for instance, from
*the G-V junction characteristics) *
is for the majority of metals in
dependent of the working func
tion in metal [12].

The extreme values drawn
in fig. 2 for the Schottky junc
tion are comparable with those
*obtained for the p-n junction at*

**F ig. ** **2. ** **Tem perature ** **dependence **
**of the resultant B 0/ A product of ****the ** **p -n****junction ** **and ** **an ** **ideal **
**Schottky junction. The experim ental **
**points for p -n junctions are taken ****from the papers [1 ], [4] ( □ ) , [7] **
**( x ) , [8 ], while those for the M S ****junctions from the papers: [9] ( O) » **

[ 10], [ 12]

### (A)

**F ig. 3. The energy hand scheme for the M S junction with the p -ty p e sem iconductor ****w ith a narrow energy gap (according to [20])**

**Temperature dependence o f the B QA product...****441**

*the temperature of 77 K. Since in the last junction the R 0A product is de*
termined by the generation-recombination processes it should be concluded

*that for the M S junction an essential contribution to the RqA product *

comes also from the space charge region. The results reported in [11] may be viewed as confirming somehow this conclusion. There, the authors no ticed that Pb-(p) PbSe junctions, at the temperature exceeding 100 K d (InR)

*/d (1 /T) an Eg(0 K) IfiJc, where p & 1.8. The value of the coefficient p is close *
to 2, which indicates the dominant contribution from the generation-recom
bination space charge of the junction [19]. Also in the paper [25] it has
been stated that the properties of the metal-(p)CdaH g 1_a.Te barrier are
*determined by the properties of the p-n junction rather than by those of *
the barrier of the ideal Schottky junction.

**The operation conditions for the photovoltaic detectors limited **
**by the background radiation (with ** **p -n**** and M -S junctions)**

The detectivity limited by the Johnson-Nyquist noise of the detector
*resistance B 0 and the noise generated by the background radiation &B *
may be determined from the formula [18]:

*D * = * f *T *

*he [ R 0A* **(10)**

*where rj is the quantum efficiency, c — light velocity, and l — wavelength *
of the incident radiation. This formula is valid for an ideal detector of
sensitivity proportional to the radiation wavelength, while the peak of
photosensitivity and the long-wave edge of sensitivity are determined
by the energy gap width. This formula takes no account of other kinds of
noise, such as 1/f. If the background radiation-limited noise is much
*greater than the Johnson-Nyquist noise (i.e. when 4 JcT/RqA <4 2q*rj&B), *
the detectivity of detector is limited by the background. In fig. 2 the curve
*fulfilling the equation 4 kT/R0A = 2q*rj&B for rj = 0.5 and 0 B is drawn *
*additionally for the view angle 2-x (dependence 0 B upon the wavelength *
corresponding to the long-wave edge of sensitivity is assumed to be consis
tent with that suggested in [26]).

*If this curve lies above the resultant curves RqA = f {T) for the photo*

voltaic detectors considered, then these detectors do not fulfil the condi tions for background-limited operation; if, however, it lies below those curves these conditions are satisfied. The intersection point of these curves occurs at the temperature ~ 150 K. Hence, it follows that for the tempera ture below 150 K the operation conditions for photovoltaic PbTe detector limited by the background radiation can be easily satisfied. This should not be expected for higher temperature.

**442** **A. Rogalski, J. Rutkowski**
**References**

**[1 ] Logothetis** **E . M ., ** **Holloway** **H ., Varga** **A . J ., Johnson** **W . J ., A p p l. P h ys. **
**L e tt. 21 (1 97 2), 411.**

**[2 ] Donnelly** **J. P ., Harman** **T . C ., S olid-St. Electron. 18 (1 97 5), 1144.**

**[3 ] Lopez-Ohero** **A ., ** **Hass** **L . D ., JantschW . , Lischka** **K ., A p p l. P h ys. L e tt. 28 **
**(1976), 546.**

**[4 ] Donnelly** **J. P ., Harman** **T . G,. Foyt** **A . G., Lindley** **W . T ., J . N on m etals 1 **
**(1 973), 123.**

**[5 ] Eddollis** **D . V ., Infrared P h ys. 16 (1 976), 47.**
**[6 ] KiliasJ ., B iu l. W A T 27 (1978), 141.**

**[7] Gooch** **C. H., Tarry H. A., Bottomley** **R . C ., Astles** **M . G., Waldock B., **

**E lectron. L e tt. 1 4 (1978), 209.**

**[8] Holloway H., Yeung K. F., A p p l. Phys. Lett. 30 (1977), 210.**

**[9 ] NillK . W ., Calaw aA . R ., Herman** **T . C ., A p p l. P h y s. L e tt. 16 (1970), 375.**
**[1 0 ] Logothetis** **E . M ., Holloway** **H ., Varga** **A . J ., Wilkes** **E ., A p p l. P h ys. L e tt. **

**19 (1 971), 318.**

**[1 1 ] HohnkeD . K ., Holloway** **H ., A p p l. P h y s. L e tt. 24 (1974), 633.**
**[1 2 ] Baars** **J ., Bassett** **D ., Schulz** **M ., P h ys. Status Sol. (a) 49 (1978), 483.**
**[1 3 ] Rogalski** **A ., Infrared P h ys. (to be published).**

**[1 4 ] Preier** **H ., Infrared P h ys. 18 (1978), 43.**

**[1 5] Smith** **R . A ., Półprzewodniki, P W N , W a rszaw a 1966, p. 85.**

**[1 6 ] MelngailisI ., Harman** **T . C ., Semiconductor and Semimetals, V o l. 5, ed, R . K . ****W illardson and A . C. Beer, A cadem ic Press, N ew Y o rk , L on don 1970, p . 111.**
**[1 7 ] EmtageP . R ., J. A p p l. P h y s. 47 (1 97 6), 2565.**

**[1 8 ] JohnsonM . R ., Chapman** **R . A ., WróbelJ. S., Infrared P h ys. 15 (1 9 7 5 ), 317.**
**[1 9] Sze****S. M ., P h ysics o f Semiconductors Devices, ed. J. W ile y and Sons, N ew Y o rk **

**1969.**

**[2 0 ] WalpoleJ. N ., NillK . W ., J. A p p l. P h y s. 42 (1971), 5609.**

**[2 1 ] Ravich Yu. I ., EfimovaB . A ., Smirnov****I . A ., M etody issledovaniya poluprovodni- ****kov v prim enenii k chalkogenidam svinca P b T e, PbSe i P b S , N au ka, M oskva ****1968.**

**[2 2] Cuff** **K . F ., Ellett** **M . R ., Kuglin** **C. D ., Williams****L . R ., P h ysics o f Semicon****ductors. Proc. 7 th Intern. Conf. D u n o d , Paris and A cadem ic Press, N ew Y o rk ****1964, pp. 6 7 7-68 4.**

**[2 3 ] Ravich Yu. I ., Efimova** **B . A ., Tamarchenko** **V . J ., P h ys. Status Sol. (b) 43 **
**(1 971), 11.**

**[2 4 ] Behrendt** **R ., Herrman** **K . H., Wandlandt** **R ., 8 th Sym posium of the IMEELO **
**Technical C om m itte on P h oton -D etectors, Praha 1978.**

**[2 5] Paw likowski** **J . M ., P h ys. Status Sol. (a) 40 (1977), 613.**

**[2 6 ] Hudson** **R . D ., Infrared S ystem Engineering, W iley-In terscien ce, N ew Y o rk , ****L on don , Sy d n ey, Toronto 1969.**

**Deceived January 3, 1980,****in revised fo rm February 1 1 ,1 9 8 0****Температурная зависимость произведения **
**фотовольтаических детекторов РЬТе**
**В работе рассчитаны предельные значения произведения Я0А диффузионных переходов ****р-п РЬТе в температурном интервале 77— 300 К . Обсуждено влияние диффузионного тока ****(для излучательной рекомбинации и рекомбинации Аугера), а также генеративно-рекомби**

**Temperature dependence o f the R^A p roduct...****443**
**национного тока на Я 0А . Расчёты произведены для оптимальных концентраций примесей ****при которых участием тоннельных составляющих тока можно пренебречь.**
**Произведены также расчёты К0А для перехода Шоттки. Результаты расчётов сопоста****влены с экспериментальными данными других авторов. Было получено хорошее соответ**
**ствие для переходов р-п. Предпринята попытка выяснения расхождения для переходов ****Шоттки. Определены рабочие режимы фотовольтаичных детекторов, обнаруживающая **
**способность которых ограничена фоновым излучением.**